The heating effect of iron-cobalt magnetic nanofluids in an alternating magnetic field: application in magnetic hyperthermia treatment
© Shokuhfar and Seyyed Afghahi; licensee Springer. 2013
Received: 15 October 2013
Accepted: 11 December 2013
Published: 20 December 2013
In this research, FeCo alloy magnetic nanofluids were prepared by reducing iron(III) chloride hexahydrate and cobalt(II) sulfate heptahydrate with sodium borohydride in a water/CTAB/hexanol reverse micelle system for application in magnetic hyperthermia treatment. X-ray diffraction, electron microscopy, selected area electron diffraction, and energy-dispersive analysis indicate the formation of bcc-structured iron-cobalt alloy. Magnetic property assessment of nanoparticles reveals that some samples are single-domain superparamagnetic, while others are single- or multi-domain ferromagnetic. The stability of the magnetic fluids was achieved by using a CTAB/1-butanol surfactant bilayer. Results of Gouy magnetic susceptibility balance experiments indicate good stability of FeCo nanoparticles even after dilution. The inductive properties of corresponding magnetic fluids including temperature rise and specific absorption rate were determined. Results show that with increasing of the nanoparticle size in the single-domain size regime, the generated heat increases, indicating the significant effect of the hysteresis loss. Finally, the central parameter controlling the specific absorption rate of nanoparticles was introduced, the experimental results were compared with those of the Stoner-Wohlfarth model and linear response theory, and the best sample for magnetic hyperthermia treatment was specified.
KeywordsFeCo alloy nanoparticles Hyperthermia treatment Specific absorption rate Microemulsion Magnetic properties Anisotropy
Magnetic nanoparticles are a topic of growing interest because of their versatile applications such as drug delivery, magnetic hyperthermia, magnetic separation, magnetic resonance imaging (MRI) contrast enhancement, and ultrahigh-density data storage[1–14]. Among those, magnetic hyperthermia is a novel therapeutic method in which the magnetic nanoparticles are subjected to an alternating magnetic field to generate a specific amount of heat to raise the temperature of a tumor to about 42°C to 46°C at which certain mechanisms of cell damage are activated[15, 16].
These mechanisms which produce heat in alternating current (AC) magnetic fields include the following: (1) hysteresis, (2) Neel or Brownian relaxation, and (3) viscous losses. The generated heat is quantitatively described by the specific absorption rate (SAR) of nanoparticles which is related to specific loss per cycle of hysteresis loop (A) by the equation SAR = A × f in which f is the frequency of the applied field.
At superparamagnetic size regime in which the hysteresis area is null, the equilibrium functions are used. In this size range depending on the anisotropy energy, the magnetic behavior of nanoparticles progressively changes from the Langevin function (L(ξ) = coth(ξ) - 1/ξ) for zero anisotropy to tanh(ξ) for maximal anisotropy where ξ = (μ 0 M s VH max)/(k B T).
- 2.Around the superparamagnetic-ferromagnetic transition size, the linear response theory (LRT) does the job for us. The LRT is a model for describing the dynamic magnetic properties of an assembly of nanoparticles using the Neel-Brown relaxation time and assumes a linear relation between magnetization and applied magnetic field. The area of the hysteresis loop is determined by (1)
In the single-domain ferromagnetic size regime, the Stoner-Wohlfarth (SW)-based models are applied which neglect thermal activation and assume a square hysteresis area that is practically valid only for T = 0 K or f → ∞ but indicates the general features of the expected properties for other conditions.
Finally, for multi-domain ferromagnetic nanoparticles, there is no simple way to model the magnetic properties of such large nanoparticles. In hyperthermia experiments, increasing the nanoparticle size to multi-domain range promotes the probability of precipitation of nanoparticles which leads to the blockage of blood vessels. Also, the larger the nanoparticle size, the higher the chance for the phagocytosis system to detect it. So, this size range has not drawn considerable attention for use in hyperthermia treatment.
The key factor to obtain the maximum SAR in conventional clinical hyperthermia treatments (f = 120 kHz, μ0Hmax =20 mT, T = 300 K) is the anisotropy of synthesized nanoparticles. Calculations of SAR as a function of anisotropy in several size regimes reveal that the maximal SAR would be obtained at the single-domain ferromagnetic size regime. So, producing high-moment magnetic nanoparticles in this range is of high value from technical and clinical aspects.
There are several works dealing with the magnetic properties of iron compounds including its oxides and alloys for use in hyperthermia treatment[14–19]. For example, Hong et al. have synthesized Fe3O4 nanoparticles using co-precipitation method and have shown that magnetic fluids of Fe3O4 nanoparticles which are coated with a surfactant bilayer feature high stability even after diluting and autoclaving and therefore are suitable for being used in magnetic hyperthermia treatment.
Among iron compounds, FeCo alloys are known to exhibit the highest magnetic properties. Iron and cobalt are both near the peak of the Slater-Pauling curve and have maximum saturation magnetization when combined together. Fe0.7Co0.3 has the highest saturation magnetization among all magnetic alloys.
Till now, several methods have been used to synthesize FeCo alloy nanoparticles which include arc discharge, polyol, hydrothermal process, RAPET, thermal decomposition, wet chemical methods[10, 11], and co-precipitation. The morphology and size distribution of as-synthesized nanoparticles are not well controlled in most of these processes. To attain the best properties for magnetic hyperthermia, the size distribution is an effective parameter. Researches show the loss of SAR due to the size distribution of nanoparticles. So, employing a method capable of producing monodisperse nanoparticles is very important. Also, stabilizing the magnetic fluid to prevent the agglomeration of nanoparticles is necessary so that the magnetic properties of the fluid would not change with time.
Among all synthetic routes, the microemulsion technique has the capability of controlling the shape, size, and size distribution of nanoparticles. In this process, the precipitation of nanoparticles takes place inside nanocages called micelles. The micelle is in the form of sphere or cylinder of oil in water (normal micelle) or water in oil (reverse micelle) which is surrounded by a layer of surfactant molecules. The morphology of micelles depends on the type of the surfactant and water-to-surfactant molar ratio (R). The technique could be used to synthesize mineral or organic compounds inside the nanoreactors. Metals or metal oxides could be produced by reduction of their mineral salts with a reductant such as borohydride.
In the present research, the shape- and size-controlled synthesis of iron-cobalt alloy nanoparticles was carried out in reverse micelles of water in hexanol, and the magnetic properties of synthesized nanoparticles were studied. Then, the magnetic fluids of each series of nanoparticles were prepared, and the stability and inductive properties of FeCo nanofluids were studied. Finally, the mechanisms of heat generation were discussed based on experimental results and theoretical models.
Iron(III) chloride hexahydrate (FeCl3 · 6H2O (%99+)), cobalt(II) sulfate heptahydrate (Co(SO4) · 7H2O (%99+)), 1-hexanol, sodium borohydride (NaBH4 (%99+)), and cetyltrimethylammonium bromide (CTAB) were purchased from MERCK chemicals (Saadat Abad, Tehran, Iran) and used as received with no further purification. High-purity nitrogen gas (%99.99+) was used to provide an oxygen-free environment during the synthesis procedure. Microemulsion 1 (ME1) and microemulsion 2 (ME2) were prepared on the basis of ternary phase diagram of water/CTAB/hexanol which is described elsewhere.
Fe0.7Co0.3 alloy nanoparticles were prepared by mixing equal volumes of ME1 and ME2 containing metal salts and precipitating agent, respectively. The [NaBH4]/[metal salts] molar ratio was kept at 2 with metal salt concentration of 0.1 M. First, ME1 was transferred into a three-necked round-bottomed flask and then ME2 was added drop by drop with vigorous stirring of ME1 under N2 atmosphere. Black precipitates of FeCo alloy nanoparticles appeared immediately after mixing of the two microemulsions. After 5 min of reaction, the synthesized nanoparticles were magnetically separated using a strong neodymium magnet, and the supernatant was decanted. Then, the nanoparticles were washed with acetone, ethanol, and chloroform several times to remove all residual elements and compounds. Some of the as-synthesized powders were annealed in a tube furnace at 623 and 823 K for 10 min under H2 atmosphere.
To maintain a magnetic fluid with stable dispersion, FeCo nanoparticles were dispersed in a vigorously stirring solution of CTAB (2 gr)/1-butanol (2 ml) in deionized water for 1 h under an inert atmosphere.
Samples and process condition
Water/surfactant molar ratio (R)
Results and discussion
Figure 3 shows an expected increase in the mean size of nanoparticles with R because as the R value increases, the relative amount of water increases and a larger micelle would be obtained; thus, the limiting stability of nanoreactors decreases, leading to larger nanoparticles. It should be noted that at R > 27, the transparent microemulsion could not form, indicating that the maximum available R for this ternary system is 27. This means that with the ternary system of water/CTAB/hexanol, the maximum achievable size for the FeCo nanoparticle is about 7 nm.
Figure 3e,f shows TEM images of the W3 sample annealed at 623 and 823 K for 10 min, respectively. It is seen that nanoparticles have grown by the fusion of smaller nanoparticles to the mean sizes of 36 and 60 nm, respectively.
Magnetic properties of FeCo nanoparticles
Magnetic properties of as-synthesized nanoparticles
Water/surfactant molar ratio (R)
Mean size (nm)
where α2 is another constant. The results obtained for A1 and A2 samples match the above proportion, indicating that annealed nanoparticles are in the multi-domain size range. The boundary between these two cases in Equations 3 and 4 is the ferromagnetic exchange length. For Fe0.7Co0.3, the values of A and K are 2.6 × 10-12 (J m-1) and 4.2 × 104 (J m-3), respectively, resulting in the exchange length of 7.86 nm. Below this size, Hc will decrease rapidly as the particle size decreases. When Hc reaches zero, nanoparticles exhibit superparamagnetic properties with a null hysteresis area as observed in the W1 sample.
Stability and inductive properties of FeCo magnetic fluids
Stability of FeCo magnetic fluids
Effect of nanoparticle size
Magnetic susceptibility of prepared fluids with various nanoparticle sizes at 32 mg/ml concentration
Nanoparticle mean size (nm)
Susceptibility (χ) × 10-5
Effect of magnetic fluid concentration
To study the effect of nanoparticle concentration on the stability of magnetic fluids, W4 nanoparticles which have the largest mean size among all samples were used to prepare magnetic fluids with different concentrations. Figure 8b shows the change of magnetic weight with time; for 32, 30, and 28 mg/ml, the magnetic weight reduces to 0.006, 0.006, and 0.005 gr, respectively. It is seen that the higher the concentration of nanoparticles, the greater the decrease of magnetic weight. In fact, at higher concentrations, nanoparticles are in lower spatial distances, and therefore, the probability of precipitation is higher based on the mechanisms described in the previous section.
Also, the effect of dilution was investigated at the ratio of 1:5 by reducing the nanoparticle concentration from 32 to 6.4 mg/ml. It is seen that the magnetic fluid is stable even after being diluted since the reduction of magnetic weight is about 0.002 gr. This is in line with the results reported by Hong et al. on the stability of Fe3O4 nanofluids. As they reported for magnetite nanoparticles, the reason is that the surfactant bilayer could not be destroyed when the magnetic fluid is diluted.
As seen from Figure 9a, the temperature increases with time and saturates after 1,800 s has elapsed, showing a behavior predicted by the Box-Lucas Equation T(t) = A(1 - e-Bt) which is often used for describing the alternating magnetic field properties of magnetic nanoparticles.
Inductive properties of prepared magnetic fluids
Mean size (nm)
Temp. rise (°C)
SAR (W g-1) (experimental)
SAR (W g-1) (SW model)
SAR (W g-1) (LRT)
≈0.84 × 10-3
≈11 × 10-3
Figure 9b indicates a direct relation of temperature rise with Hc and Ms which means that the generated heat increases by enhancing the hysteresis area, showing an important contribution of hysteresis loss to the generated heat.
where ρ = 8,300 (kg m-3) is the density of FeCo alloy, kB is the Boltzmann constant, V is the volume of nanoparticles, f = 5.5 × 10-4 (Hz) is the measurement frequency, and τ0 = 10-10 (s) is the intrawell relaxation time. Therefore, by considering the values of μ0Hc from Figure 10a,b, the anisotropy constants for W4 and W3 are calculated to be 4.1 × 104 (J m-3) and 6.64 × 104 (J m-3), respectively. Comparing the anisotropy values obtained from magnetic measurements with the optimum anisotropies from Equation 6 reveals that for the W3 sample, these two values are very close together, indicating that the maximum generated heat for this sample is around that which we obtained experimentally, but for the W4 sample, the optimum anisotropy is about 2.5 times greater than the experimental value. As the result of this deviation from the optimum value in the W4 sample (which also exhibits broader size distribution than W3 sample (see Figure 3)), the detrimental effect of nanoparticle size distribution makes the maximum achievable SAR decrease. As noted by Carrey et al., the particle size distribution has a negative effect on the maximum achievable SAR, and the anisotropy controls this effect.
Assuming f = 120 kHz, the corresponding SARs for W4 and W3 samples are 540 and 165 (W g-1), respectively. If we apply the LRT model instead, by considering τR = τN = τ0exp(KeffV/kBT), the values of SAR could be calculated from Equation 1 as seen in Table 4.
The comparative study between experimental and theoretical values of SAR indicates the following: (a) The experimental values are between pure hysteresis (SW model) and pure relaxation (LRT) which means that both loss mechanisms are involved. (b) Assuming the maximum contribution of relaxation to the total loss, for the W3 sample, the contribution of relaxation to the total SAR is 0.16% and the remaining SAR belongs to the hysteresis (99.84%), and for the W4 sample, the corresponding values are 0.76% and 99.24%, respectively, indicating that hysteresis is a more effective mechanism in producing of heat. (c) W4 ferromagnetic nanoparticles exhibit higher experimental and theoretical SAR compared with other samples. As noted by Lacroix et al., given the weak magnetic fields in hyperthermia treatment, the maximum SAR would be obtained for soft ferromagnetic nanoparticles or the nanoparticles near the superparamagnetic transition. This is consistent with our experimental results.
Size-controlled synthesis of FeCo nanoparticles was done using microemulsion method. It was observed that by increasing the water-to-surfactant molar ratio, the nanoparticles become larger. The maximum size of nanoparticles in the ternary system of water/CTAB/hexanol is about 7 nm. Size dependency of magnetic properties including Ms and Hc was investigated. The observed increase in Ms with size is due to disappearance of the magnetic dead layer in larger nanoparticles. However, the observed change in coercivity with size is due to transition between various size regimes and consequently the magnetization reversal mechanisms. The nanoparticles were stabilized using a CTAB/1-butanol bilayer. The stability of nanoparticles was studied at various nanoparticle sizes and concentrations. Results show that by increasing the nanoparticle size or concentration, the stability of the magnetic fluid decreases due to magnetic interaction and consequent aggregation of nanoparticles.
The inductive properties of nanoparticles such as temperature rise and specific absorption rate were evaluated at various nanoparticle sizes and were observed to have direct relation with the size of nanoparticles. Both Hc and SAR show similar tendencies of changing with particle size. The reason lies in anisotropy as a central parameter controlling both Hc and SAR.
Only W4 and W3 ferromagnetic nanoparticles are found to be capable of being used in hyperthermia treatment which passed the minimum temperature rise of 5°C to 9°C. The comparison of experimental results with those of Stoner-Wohlfarth and LRT models shows that hysteresis and relaxation mechanisms are both involved in the generation of heat, but the contribution of hysteresis is far greater than relaxation.
The authors would like to thank Mr. B. Saberi for his great help in providing the requested facilities of this work.
- Hong RY, Li JH, Li HZ, Ding J, Zheng Y, Wei DG: Synthesis of Fe3O4 nanoparticles without inert gas protection used as precursors of magnetic fluids. J Magn Magn Mater 2008, 320: 1605–1614. 10.1016/j.jmmm.2008.01.015View ArticleGoogle Scholar
- Suresh G, Saravanan P, Babu DR: One-pot synthesis of Fe-Co nanospheres by modified polyol process and their structural, magnetic studies. J Phys, Conference Series 2011, 292: 012015.View ArticleGoogle Scholar
- Feng B, Hong RY, Wang LS, Guo L, Li HZ: Synthesis of Fe/APTES/PEG diacid functionalized magnetic nanoparticles for MR imaging. Colloid Surf A 2008, 328: 52–59. 10.1016/j.colsurfa.2008.06.024View ArticleGoogle Scholar
- Nguyen Q, Chinnasamy CN, Yoon SD, Sivasubramanian S, Sakai T, Baraskar A, Mukerjee S, Vittoria C, Harris VG: Functionalization of FeCo alloy nanoparticles with highly dielectric amorphous oxide coatings. J Appl Phys 2008, 103: 07D532.Google Scholar
- Hong RY, Li JH, Zhang SZ, Li HZ, Zheng Y, Ding JM, Wei DG: Preparation and characterization of silica-coated Fe3O4 nanoparticles used as precursor of ferrofluids. Appl Surf Sci 2009, 255: 3485–3492. 10.1016/j.apsusc.2008.09.071View ArticleGoogle Scholar
- Jae Lee S, Cho JH, Lee C, Cho J, Kim YR, Park JK: Synthesis of highly magnetic graphite-encapsulated FeCo nanoparticles using a hydrothermal process. Nanotechnology 2011, 22: 375603. 10.1088/0957-4484/22/37/375603View ArticleGoogle Scholar
- Holodelshikov E, Perelshtein I, Gedanken A: Synthesis of air stable FeCo/C alloy nanoparticles by decomposing a mixture of the corresponding metal-acetyl acetonates under their autogenic pressure. Inorg Chem 2011, 50: 1288–1294. 10.1021/ic101825eView ArticleGoogle Scholar
- Li JH, Hong RY, Li HZ, Ding J, Zheng Y, Wei DG: Simple synthesis and magnetic properties of Fe3O4/BaSO4 multi-core/shell particles. Mater Chem Phys 2009, 113: 140–144. 10.1016/j.matchemphys.2008.07.054View ArticleGoogle Scholar
- Lee GH, Huh SH, Jeong JW, Kim SH, Choi BJ, Jeong JH: Structural and magnetic properties of bimetallic FeCo nanoclusters. J Kor Phys Soc 2003, 42(3):367–370.Google Scholar
- Guo Z, Henry LL, Podlaha EJ: CoFe, Fe and Co nanoparticles displacement with Cu ions. ECS Transactions. ECS T 2007, 3(25):337–345.View ArticleGoogle Scholar
- Wei XW, Zhu GX, Liu YJ, Ni YH, Song Y, Xu Z: Large-scale controlled synthesis of FeCo nanocubes and microcages by wet chemistry. Chem Mater 2008, 20: 6248–6253. 10.1021/cm800518xView ArticleGoogle Scholar
- Hong RY, Feng B, Chen LL, Liu GH, Li HZ, Zheng Y, Wei DG: Synthesis, characterization and MRI application of dextran-coated Fe3O4 magnetic nanoparticles. Biochem Eng J 2008, 42: 290–300. 10.1016/j.bej.2008.07.009View ArticleGoogle Scholar
- Shin SJ, Kim YH, Kim CW, Cha HG, Kim YJ, Kang YS: Preparation of magnetic FeCo nanoparticles by coprecipitation route. Curr Appl Phys 2007, 7: 404–408. 10.1016/j.cap.2006.09.012View ArticleGoogle Scholar
- Timothy LK, Xu YH, Ying J, Wang JP: Biocompatible high-moment FeCo-Au magnetic nanoparticles for magnetic hyperthermia treatment optimization. J Magn Magn Mater 2009, 321: 1525–1528. 10.1016/j.jmmm.2009.02.079View ArticleGoogle Scholar
- Kumar CSSR, Mohammad F: Magnetic nanomaterials for hyperthermia-based therapy and controlled drug delivery. Adv Drug Deliver Rev 2011, 63: 789–808. 10.1016/j.addr.2011.03.008View ArticleGoogle Scholar
- Wang YM, Cao X, Liu GH, Hong RY, Chen YM, Chen XF, Li HZ, Xu B, Wei DG: Synthesis of Fe3O4 magnetic fluid used for magnetic resonance imaging and hyperthermia. J Magn Magn Mater 2011, 323: 2953–2959. 10.1016/j.jmmm.2011.05.060View ArticleGoogle Scholar
- Carrey J, Mehdaoui B, Respaud M: Simple models for dynamic hysteresis loop calculations of magnetic single-domain nanoparticles: application to magnetic hyperthermia optimization. J Appl Phys 2011, 109: 083921. 10.1063/1.3551582View ArticleGoogle Scholar
- Lacroix LM, Malaki RB, Carrey J, Lachaize S, Respaud M, Goya GF, Chaudret B: Magnetic hyperthermia in single-domain monodisperse FeCo nanoparticles: evidences for Stoner–Wohlfarth behavior and large losses. J Appl Phys 2009, 105: 023911. 10.1063/1.3068195View ArticleGoogle Scholar
- Liu G, Hong RY, Guo L, Liu GH, Feng B, Li YG: Exothermic effect of dextran-coated Fe3O4 magnetic fluid and its compatibility with blood. Colloid Surf A: Physicochem Eng Aspects 2011, 380: 327–333. 10.1016/j.colsurfa.2011.03.006View ArticleGoogle Scholar
- Gubin SP, Koksharov YA, Khomutov GB, Yurkov GY: Magnetic nanoparticles: preparation, structure and properties. Russ Chem Rev 2005, 74(6):489–520. 10.1070/RC2005v074n06ABEH000897View ArticleGoogle Scholar
- Destrée C, Nagy JB: Mechanism of formation of inorganic and organic nanoparticles from microemulsions. Adv Colloid Intefac 2006, 123: 353–367.View ArticleGoogle Scholar
- Quintela MAL: Synthesis of nanomaterials in microemulsions: formation mechanisms and growth control. Curr Opin Colloid Interf Sci 2003, 8: 137–144. 10.1016/S1359-0294(03)00019-0View ArticleGoogle Scholar
- Espí RM, Weiss CK, Landfester K: Inorganic nanoparticles prepared in miniemulsion. Opin Colloid Interf Sci 2012, 17: 212–224. 10.1016/j.cocis.2012.04.002View ArticleGoogle Scholar
- Schork FJ, Luo Y, Smulders W, Russum JP, Butte A, Fontenot K: Miniemulsion polymerization. Adv Polym Sci 2005, 175: 129–255. 10.1007/b100115View ArticleGoogle Scholar
- Tamamushi BI: Colloid and surface chemical aspects of mesophases (liquid crystals). Pure & Appl Chem 1976, 48: 441–447. 10.1351/pac197648040441View ArticleGoogle Scholar
- Sharifi I, Shokrollahi H, Doroodmand MM, Safi R: Magnetic and structural studies on CoFe2O4 nanoparticles synthesized by co-precipitation, normal micelles and reverse micelles methods. J Magn Magn Mater 2012, 324: 1854–1861. 10.1016/j.jmmm.2012.01.015View ArticleGoogle Scholar
- Andrade AL, Fabris J, Ardisson J, Valente MA, Ferreira JMF: Effect of tetramethylammonium hydroxide on nucleation, surface modification and growth of magnetic nanoparticles. J Nanomater 2012, 454759.Google Scholar
- Miller JT, Kropf AJ, Zhac Y, Regalbutoc JR, Delannoy L, Louis C, Bus E, van Bokhoven JA: The effect of gold particle size on Au–Au bond length and reactivity toward oxygen in supported catalysts. J Catal 2006, 240: 222–234. 10.1016/j.jcat.2006.04.004View ArticleGoogle Scholar
- Chen DX, Pascu O, Roig A, Sanchez : Size analysis and magnetic structure of nickel nanoparticles. J Magn Magn Mater 2010, 322: 3834–3840. 10.1016/j.jmmm.2010.07.046View ArticleGoogle Scholar
- Herzer G: Nanocrystalline soft magnetic materials. J Magn Magn Mater 1992, 112: 258–262. 10.1016/0304-8853(92)91168-SView ArticleGoogle Scholar
- Liu X, Sooryakumar R, Gutierrez CJ, Prinz GA: Exchange stiffness and magnetic anisotropies in bcc Fe1-x Cox alloys. J Appl Phys 1994, 75: 7021. 10.1063/1.356763View ArticleGoogle Scholar
- Tian Y, Yu B, Li X, Li K: Facile solvothermal synthesis of monodisperse Fe3O4 nanocrystals with precise size control of one nanometre as potential MRI contrast agents. J Mater Chem 2011, 21: 2476–2481. 10.1039/c0jm02913kView ArticleGoogle Scholar
- Cabañas BM, Leclercq S, Barboux P, Fédoroff M, Lefèvre G: Sorption of nickel and cobalt ions onto cobalt and nickel ferrites. J Colloid Interf Sci 2011, 360: 695–700. 10.1016/j.jcis.2011.04.082View ArticleGoogle Scholar
- Sun S: Recent advances in chemical synthesis, self-assembly, and applications of FePt nanoparticles. Adv Mater 2006, 18: 393–403. 10.1002/adma.200501464View ArticleGoogle Scholar
- Mørup S, Hansen MF, Frandsen C: Magnetic interactions between nanoparticles. Beilstein J Nanotechnol 2010, 1: 182–190.View ArticleGoogle Scholar
- Murase K, Takata H, Takeuchi Y, Saito S: Control of the temperature rise in magnetic hyperthermia with use of an external static magnetic field. Physica Medica 2013, 29: 624–630. 10.1016/j.ejmp.2012.08.005View ArticleGoogle Scholar
- Ohnuma I, Enokia H, Ikeda O, Kainuma R, Ohtani H, Sundman B, Ishida K: Phase equilibria in the Fe–Co binary system. Acta Mater 2002, 50: 379–393. 10.1016/S1359-6454(01)00337-8View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.